Materials 2014, 7, 59345958; doi:10.3390/ma7085934 OPEN ACCESS
materials ISSN 19961944 www.mdpi.com/journal/materials Article
Experimental Study on the Seismic Performance of Recycled Concrete Brick Walls Embedded with Vertical Reinforcement Wanlin Cao, Yongbo Zhang, Hongying Dong *, Zhongyi Zhou and Qiyun Qiao College of Architecture and Civil Engineering, Beijing University of Technology, Beijing 100124, China; EMails:
[email protected] (W.C.);
[email protected] (Y.Z.);
[email protected] (Z.Z.);
[email protected] (Q.Q.) * Author to whom correspondence should be addressed; EMail:
[email protected]; Tel./Fax: +861067396617. Received: 11 June 2014; in revised form: 6 August 2014 / Accepted: 6 August 2014 / Published: 19 August 2014
Abstract: Recycled concrete brick (RCB) is manufactured by recycled aggregate processed from discarded concrete blocks arising from the demolishing of existing buildings. This paper presents research on the seismic performance of RCB masonry walls to assess the applicability of RCB for use in rural lowrise constructions. The seismic performance of a masonry wall is closely related to the vertical load applied to the wall. Thus, the compressive performance of RCB masonry was investigated firstly by constructing and testing eighteen RCB masonry compressive specimens with different mortar strengths. The loadbearing capacity, deformation and failure characteristic were analyzed, as well. Then, a quasistatic test was carried out to study the seismic behavior of RCB walls by eight RCB masonry walls subjected to an axial compressive load and a reversed cyclic lateral load. Based on the test results, equations for predicting the compressive strength of RCB masonry and the lateral ultimate strength of an RCB masonry wall were proposed. Experimental values were found to be in good agreement with the predicted values. Meanwhile, finite element analysis (FEA) and parametric analysis of the RCB walls were carried out using ABAQUS software. The elasticplastic deformation characteristics and the lateral loaddisplacement relations were studied. Keywords: recycled concrete brick (RCB); compressive performance; seismic performance; experimental study; numerical simulation
Materials 2014, 7
5935
1. Introduction China is a large resource consumer because of the rapid growth of its economics and environmental issues. According to statistics, the consumption of cement in China is 820 million tons and accounts for 55% of the world’s consumption. It is estimated that about 200 million tons of waste concrete are produced each year in the mainland of China [1]. Recycling and reusing construction waste has become one of the key issues that should be solved urgently in China with the rapid urbanization, new countryside construction and largescale urban renewal. In view of environmental protection, the conservation of natural resources and the shortage of lands for waste disposal, traditional clay brick has been forbidden by China’s government. There is thus an urgent need to develop new brick suitable for residential buildings in view of masonry structures that are still playing a significant role in rural lowrise constructions. The difficulties of the disposal of discarded concrete blocks and demolition waste with a developing scarcity of virgin aggregate have appealed to the use of recycled aggregate instead of natural aggregate. Crushed concrete rubble, after separation from other waste and being sieved, can be used as a substitute for natural coarse aggregates in concrete or as a subbase or a base layer in pavements [2–5]. This type of recycled material is called recycled aggregate. Recycled aggregate can roughly be divided into two categories, namely recycled coarse aggregate and recycled fine aggregate. The recycled concrete bricks molded with recycled aggregate are suitable for rural lowrise constructions. Previous research has focused on the material performance, mechanics performance and seismic performance of recycled aggregate concrete structures and has accumulated many achievements. The research of recycled concrete brick has been little studied, especially the seismic design of an RCB wall structure in rural lowrise constructions. In fact, an attempt has been made by Collins et al. [6] to use recycled aggregates in making blocks for a beamandblock floor system. The blocks were 440 mm × 215 mm × 100 mm in dimension and were produced at a block factory. Recycled aggregates were used to replace 25%–75% by weight of the natural aggregate (including coarse and fine aggregates). A compressive strength of 6.75 MPa and a transverse strength of 1.23 MPa were reported for the blocks, with 75% of the natural aggregates replaced by recycled aggregates. Poon et al. [7] studied the applicability of recycled aggregates in molded recycled concrete bricks and blocks by their compressive and bending performance test, including their compressive strength, transverse strength, shrinkage, skid resistance and density. Results showed that the replacement of coarse and fine natural aggregates by recycled aggregates at the levels of 25% and 50% had little effect on the compressive strength of the bricks and blocks, but higher levels of replacement reduced the compressive strength. The compressive strength of recycled concrete brick decreased when the recycled aggregate substitution ratio exceeded 50%. Gu et al. [8] tested the mechanical performance of recycled concrete brick walls under repeated loading and analyzed the bearing capacity and failure process of recycled concrete brick walls. Cao et al. [9] tested the seismic performance of the RCB masonry structure by the shake table test of two RCB masonry buildings with or without vertical reinforcement. Results have shown that an RCB masonry building with vertical reinforcement exhibited better seismic performance and a lighter degree of damage than that of the ordinary RCB masonry building. He et al. [10] studied the compressive and bending performance of RCB with a compressive strength range from 15 to 30 MPa. The impact of recycled aggregate on the solid concrete brick mechanical
Materials 2014, 7
5936
properties and physical properties was analyzed. Guo et al. [11] investigated the seismic performance of recycled concrete perforated brick masonry subjected to low frequency reversed cyclic load. The test results show that the seismic performance of recycled concrete perforated brick masonry is similar to those of ordinary concrete perforated brick walls with good hysteresis loops and ductility, as well as strong energy dissipation capacities. He et al. [12] studied the drying shrinkage performance of solid concrete bricks made from recycled coarse aggregate. Results showed that recycled aggregate can increase the shrinkage of solid concrete brick. The shrinkage of recycled solid concrete bricks (fully substituted) is larger than ordinary concrete bricks by 1.6–2 times. A water reducer is helpful to improve the water retention and decrease the shrinkage of brick. Valdés et al. [13] investigated the physical and mechanical properties of concrete bricks produced with recycled aggregates. The results show that the compressive strength of the concrete bricks manufactured with recycled material showed resistances of 15% lower than those manufactured with natural aggregates. In view of the shortcomings of previous studies, it is worthwhile to investigate the seismic performance of RCB masonry walls in order to prompt a better application in rural lowrise constructions. It has been known that the seismic performance of masonry walls is closely related to the vertical load applied on the wall. So far, a variety of studies has been carried out to study the shearcompression ratios and the failure criterion of masonry. These studies were all based on common brick masonry without reinforcement. Lourenco et al. [14] analyzed the horizontal force and horizontal displacement relations, and failure criterion expressions were proposed, as well. It is stated that the failure model of masonry can be divided into two types: Tensioncontrolled failure and compressioncontrolled failure. The proposed failure criterion expressions cannot explain the failure that may occur in a masonry structure. The failure criterion that is proposed by Andreaus [15] can explain all of the failure patterns of masonry, including tensioncontrol, compressioncontrol and slidingcontrol failure; however, it was too complex to implement. Shi [16] pointed out that the failure models of a masonry wall depended on the size of the vertical load and can be classified as shearfriction, shearcompression and diagonal compression. Luo et al. [17] tested the shear performance of masonry and achieved shearcompression correlation curves. Studies have shown that the shear strength of masonry increased with the axial stress ratio increasing in the range of 0–0.6, but the increasing gradient becomes smaller. When the axial stress ratio exceeded 0.6, the shear strength of masonry dropped rapidly and, then, down to zero when the axial stress ratio reached 1.0. The shearcompression correlation curve of masonry proposed by Cai et al. [18] showed that the shear strength of masonry reached the maximum value when the axial stress ratio was equal to 0.475. Liu et al. [19] established the failure criterion of masonry in shearcompression on the basis of mechanic principles and a statistical method. A calculation method of shear strength by the failure criterion was proposed, as well. It pointed out that the axial stress ratio of 0.32 was the boundaries between shear sliding failure and tensile failure and the axial stress ratio of 0.67 was between tensile failure and compression failure. Therefore, to study the seismic performance of RCB masonry walls, we first need to explore the compressive performance of RCB masonry. To investigate the applicability of RCB masonry in rural lowrise constructions extensively, two critical technical problems of RCB masonry were investigated, the compressive performance and the seismic performance. The compressive performance was studied first based on eighteen RCB compressive specimens with different mortar strengths under vertical load. The compressive strength,
Materials 2014, 7
5937
deformation and failure characteristic were analyzed. Then, the seismic performance was investigated based on eight RCB masonry walls with different parameters under reversed cyclic lateral loads. Their seismic performance was comparatively analyzed. Furthermore, an elasticplastic finite element analysis (FEM) and parametric analysis of the RCB masonry walls were carried out by ABAQUS software. The elasticplastic deformation characteristics and the relationships of lateral load to top displacement were studied. The proposed approach, which is named recycled concrete brick walls embedded with vertical reinforcement, has had a national invention patent applied for and authorized. The paper aims to investigate its superiority to traditional approaches that are accepted internationally and to explore its applicability in rural areas. 2. Experimental Section 2.1. Compressive Performance of RCB Masonry 2.1.1. Materials and Specimen Preparation The RCB was manufactured by a mechanized molding machine in Beijing (YuanTaiDa Environmental Protection Building Materials Technology Limited Liability Company of China). Table 1 shows the mix proportions for recycled concrete bricks. The cementitious materials used were an ordinary Portland cement (P·O 42.5) complying with GB1752007 [20]. The recycled aggregates were C&D (Construction and Demolition) wastes sourced from a demolished house in Beijing. Then, the C&D wastes underwent a further process of mechanized crushing and sieving to produce fine aggregate and coarse aggregate in the factory mentioned above. The marl, containing some clay, was a kind of precipitate particle obtained from the sedimentation tank after the recycled aggregates were rinsed by water. The fly ash was a kind of fine powder, which was collected by the aspiration air separation system during the production process of the recycled aggregate. The mixed materials are molded under a combined vibrating and compacting action. Then, the bricks were removed from the molds and cured in air at room temperature for 28 days. The measured average compressive strength of 28 days for the RCB was 7.9 MPa. Table 1. Mix proportions for recycled concrete bricks. RCB: recycled concrete brick. Mix Notation RCB
Cement 143
Proportion (kg) Recycled Fine Aggregate Marl Fly Ash Added Water 608 152 240 120
Eighteen RCB masonry compressive specimens with different mortar strengths were designed and tested under a vertical load. The specimens contained three groups, which were called A, B and C, respectively, corresponding to the designed mortar strength of M5, M7.5 and M10. Each group contained six specimens. KYM 51–KYM 56 were designed with a mortar strength of 5 MPa in Group A. KYM 7.51–KYM 7.56 were designed with a mortar strength of 7.5 MPa in Group B, and KYM 101–KYM 106 were designed with a mortar strength of 10 MPa in Group C (KYM stand for the compressive masonry in Chinese). The dimensions of all of the RCB masonry specimens were 780 mm × 260 mm × 390 mm. The dimensions of the RCB brick were 53 mm × 115 mm × 260 mm.
Materials 2014, 7
5938
The measured average mortar strengths of 28 days for Groups A–C were 4.84, 7.33 and 9.44 MPa, respectively. The details of the compressive specimen are shown in Figure 1. The compressive strength of masonry is affected by certain factors, such as the size and shape of the masonry, the loading method, and so on. The crosssection size of standard brick masonry specimen adopted by the former Soviet Union is 370 mm × 490 mm. RILEM (International Union of Laboratories and Experts in Construction Materials, Systems and Structures) recommends a onestoryheight brick wall or brick column as a standard brick masonry specimen. The United States, Canada and Australia adopt a prism piled up by laying bricks or stones as the brick masonry standard specimen. While in China, the standard crosssection size of brick masonry is 240 mm × 370 mm, the ratio of the masonry height to the short length of the crosssection is smaller than 2.5–3.0. This results in determining the current specification of brick masonry compression strength. The strength conversion coefficient is calculated by Equation (1) [16] when the brick masonry has a nonstandard cross section.
1
ψ
0.72
20 s A
(1)
where ψ is the strength conversion coefficient, S is the perimeter of the nonstandard crosssection and A is the area of the nonstandard crosssection. Thus, considering the RCB size, we adopted the crosssection of the specimens by 780 mm × 260 mm × 390 mm. Figure 1. The section details of the compressive specimen: (a) facade size; (b) Section 11; (c) Section 22. (Unit: millimeters).
390
390
260
11
2
(a)
780
1
1
780
260
2
22
(b)
(c)
2.1.2. Test Setup and Loading Procedure The specimens were tested according to the standard test method of the basic mechanics properties of masonry (GB/T 501292011) [21]. The vertical load was applied by steps, and the value of each step was 10% of the predicted failure load. The load of each step was applied completely within 1–1.5 min and maintained for 1–2 min before the next step. When the total load value reached 80% of the predicted failure load, continuous load was applied with the original load speed until the specimens were damaged. The maximum load value, which is read from the testing machine, was the failure load of the specimen. Dial indicators were set at the two long sides of the specimen to monitor the axial
Materials 2014, 7
5939
compressive and lateral expansive deformation, with a gauge length of 280 mm and 210 mm, respectively. The test setup and dial indicator arrangement are illustrated in Figure 2. Figure 2. (a) Test setup; (b) Dial indicator arrangement.
(a)
(b)
2.1.3. Failure Characteristics The failure process of RCB masonry contained two stages. The first stage was from the start to the occurrence of the first crack. With the increase of the load, the first crack appeared in the vertical mortar joint at the top of the short edge. The second stage was from crack to failure. With the increase of the load, cracks at the short edge developed downwards along the vertical mortar joint and penetrated at the lower part of the masonry gradually. Meanwhile, vertical cracks also appeared in the center of the long edge and developed gradually, until the specimens cracked. The failure process of the three groups of specimens is as follows: (1) Six specimens of Group A: Due to the setting deviation and asymmetry load, the corner of KYM51 crushed first, because of compression, and then, the specimen cracked; as for the remaining five specimens, the first crack appeared in the vertical mortar joint at the top of the short edge, then vertical cracks also appeared at the long edge. With the increase of the load, cracks developed gradually until they were through the wall, and finally, the specimens cracked; (2) Six specimens of Group B: As for specimen KYM7.54, the first crack appeared in the vertical mortar joint in the middle of the short edge and developed rapidly as the load increased, its top corner crushed, then the specimen cracked; as for the other five specimens, the failure process was similar to the specimens of Group A, the difference being that the bearing capacity increased with the improvement of the mortar strength; (3) Six specimens of Group C: The failure process was also similar to specimens of Groups A and B; the bearing capacity was higher, because of the higher mortar strength. The typical failure characteristics of these three group specimens are shown in Figure 3. 2.1.4. Measured Compressive Strength The measured cracking load, failure load and compressive strength of the specimens are listed in Table 2, where Pc is the cracking load, Pu is the failure load and fc,m is the average compressive strength. In the specimen named KYM ij, KYM stand for the compressive masonry in Chinese; i represents the designed mortar strength grade of each group, namely, i equals 5, 7.5 and 10,
Materials 2014, 7
5940
representing Groups A, B and C, respectively. j represents the number of the specimens in each group. It points out that three specimens of group C were cured outdoors in the winter due to the space constraints and were damaged for a certain reason, while other specimens were cured indoors. Thus, the first 3 results for Group C are missing from Table 2. It can be seen from Table 2 that the cracking load and failure load of RCB masonry increased as the mortar strength increased. The mortar strength was a critical factor for the compressive strength of the RCB masonry. Figure 3. Typical failure characteristics: (a) KYM55; (b) KYM7.53; (c) KYM106.
(a)
(b)
(c)
Table 2. Measured cracking load, failure load and compressive strength of specimens. Group A Specimen
Group B
Group C
cracking
failure
compressive
cracking
failure
compressive
cracking
failure
compressive
load Pc
load Pu
strength fc,m
load Pc
load Pu
strength fc,m
load Pc
load Pu
strength fc,m
(kN)
(kN)
(MPa)
(kN)
(kN)
(MPa)
(kN)
(kN)
(MPa)
KYM i1
139
215
2.12
145
225
2.22



KYM i2
128
196
1.93
192
288
2.84



KYM i3
148
224
2.21
165
255
2.51



KYM i4
122
187
1.84
198
305
3.01
241
365
2.83
KYM i5
144
224
2.21
133
204
2.01
231
346
2.89
KYM i6
113
173
1.71
125
192
1.89
221
335
2.81
Average
132
203
2.00
160
245
2.41
231
348
2.84
2.1.5. Compressive Strength Calculation The compressive strength of common clay brick has been studied by some scholars locally and abroad. In general, brick strength and mortar strength are two critical factors that influence the compressive strength of brick masonry. Calculated equations have been proposed for brick masonry compressive strength based on the identification of theory and experience. The representative theoretical equations were presented by Francis [22], Hilsdorf [23] and Hendry [24]. The theoretical equations presented by Francis and Hilsdorf were deduced based on a prism piled up by laying bricks. It cannot reflect the elastoplastic performance of masonry material and remains to be further researched. Hendry has made some supplements to the above derivation method adopted by Francis and Hilsdorf. The biaxial compressiontension performance of brick and the triaxial compression
Materials 2014, 7
5941
performance of mortar were studied by Hendry to make up the deficiency of the assumption adopted by Francis and Hilsdorf. The representative empirical equations were presented by Oнищик [25] and Grimm [26]. The equation presented by Oнищик has taken into consideration the primary factors affecting the masonry compressive strength, but the calculation is relatively complicated with more parameters. Furthermore, considering the primary factors affecting the masonry compressive strength, the equation presented by Grimm had a great limitation and was only suitable for the calculation of brick masonry prism compressive strength. The equation adapted by British Standards [27] and ISO/TC179 for the calculation of masonry compressive strength was simpler by form, but did not match with reality. Compared with other equations widely used internationally, Equation (2) [16], as below, for the calculation of average compressive strength of masonry was adapted by the current design code of masonry structures (GB500032011) in China.
f m k1 f1α (1 0.07 f 2 )k2
(2)
where fm is the average compressive strength of masonry (MPa), f1 is the average compressive strength of the block (MPa), f2 is the average compressive strength of mortar, k1 is a parameter related to the type of block and construction method, α is a parameter related to the height of block and k2 is a correction coefficient of compressive strength related to the lowstrength mortar, when f2 ≥ 1.0, k2 = 1.0. The parameters k1 = 0.78, α = 0.5 and k2 = 1.0 when calculating the average compressive strength of common clay brick masonry. In this paper, we adopt Equation (2) and the parameters k1 = 0.55, α = 0.5 and k2 = 1.0 for the calculation of the RCB masonry average compressive strength, and the strength conversion coefficient ψ is related, as well. Table 3 compares the calculated values by Equation (2) with the measured values. It can be seen that the calculation results agree well with the experimental results. Equation (2) with appropriate parameters can be used to predict the average compressive strength of RCB masonry. Table 3. Comparison of average compressive strength between calculated values and measured values. Groups A B C
f1 (MPa) 7.90 7.90 7.90
f2 (MPa) 4.84 7.33 9.44
Calculated Values (MPa) 2.12 2.40 2.63
Measured Values (MPa) 2.00 2.41 2.84
Errors (%) 5.98 0.60 7.41
2.1.6. Elastic Modulus and Poisson’s Ratio Figure 4 shows the measured axial stressaxial strain curves of different mortar strengths. It shows that the stressstrain curves were nearly linear before reaching the failure load. The compressive strength of the RCB masonry increased as the mortar strength increased. The elastic modulus of RCB masonry takes the secant modulus, where the stress σ equals 0.4 fm. The measured elastic modulus E and Poisson’s ratio ν are listed in Table 4. Table 4 shows that the elastic modulus and Poisson’s ratio of the RCB masonry increase with the increase of the mortar strength.
Materials 2014, 7
5942
Figure 4. Measured axial stressaxial strain curves of different mortar strengths. (a) Group A; (b) Group B; (c) Group C; (d) Average stressaxial strain curves of different mortar strengths.
(a)
(b)
(c)
(d)
Table 4. Elastic modulus and Poisson’s ratio. Group A B C
f1 (MPa) 7.90 7.90 7.90
f2 (MPa) 4.84 7.33 9.44
fm (MPa) 2.00 2.41 2.84
ν 0.162 0.176 0.191
E (MPa) 2761.5 3069.7 3320.4
2.2. Seismic Performance of RCB Masonry Walls 2.2.1. Materials and Specimen Preparation The measured tensile yield strength of the vertical reinforcement (hotrolled ribbed steel bar and a diameter of 20 mm) and the Ushaped horizontal reinforcement (hotrolled plain steel bar and a diameter of 4 mm) were 375 and 312 MPa, respectively. The measured prism compressive strength of fine aggregate concrete was13.4 MPa, while the measured compressive strength of RCB and mortar were 7.90 and 7.44 MPa, respectively. Eight RCB masonry walls with heighttowidth aspects ratios of 0.6 and 1.0 were fabricated and tested under reversed cyclic loading. The specimens can be divided into four groups according to the wall thickness and heighttowidth aspects ratio. The variables involved included the wallpanel aspect
Materials 2014, 7
5943
ratio, wall thickness, distribution of vertical reinforcement and the axial compressive load. Specimen details are summarized in Table 5. In the second column of Table 5, the letters MWA and MWB in the specimen labels stand for the masonry wall without vertical reinforcement and the masonry wall with vertical reinforcement, respectively. The number that follows (1, 2, 3, and 4) is the number of the group. Table 5. Details of the specimens. Group Group 1 Group 2 Group 3 Group 4
Specimen
HeighttoWidth Aspect Ratios
Wall Thickness (mm)
Number of Vertical Reinforcement
Axial Compressive Force (kN)
MWA1 MWB1 MWA2 MWB2 MWA3 MWB3 MWA4 MWB4
0.6 0.6 1.0 1.0 0.6 0.6 1.0 1.0
260 260 260 260 390 390 390 390
0 3 0 2 0 3 0 2
348 348 245 245 522 522 367 367
The size of RCB was 260 mm × 115 mm × 53 mm. The vertical reinforcement was arranged in the center of 100 mm × 100 mm square holes, which were formed by specially shaped bricks and distributed symmetrical on the crosssection of the wall. Fine aggregate concrete was cast into the square holes to form concealed columns. Moreover, vertical reinforcement was arranged at both ends of the wall as a priority and, then, in the center, when the wall was too long. Three vertical steel bars were set separately at both ends and the center of the specimens, MWB1 and MWB3. Two vertical steel bars were set separately at both sides of the specimens, MWB2 and MWB4. The distance from the centroid of vertical reinforcement to the nearby end edge of the wall was 130 mm. The roots of vertical steel bars were anchored into the base of specimens. The vertical reinforcement was connected with the wall by a Ushaped horizontal reinforcement every six brick units. Details of the geometry and reinforcement are shown in Figure 5. The settings of the vertical reinforcement are shown in Figure 6. Figure 5. The dimensions of all of the specimens: (a) MWA1; (b) MWB1; (c) MWA2; (d) MWB2; (e) MWA3; (f) MWB3; (g) MWA4; (h) MWB4. (Unit: millimeters) 100
100
(a)
2
455
1890 2800
455
1890
11
20
1890 2800 1890
11
2690
1890
22
22
(b)
455
1 2
260
2690
305
1 2 20
(c)
11
260
260
2690 3300
100
400 1
2
260
2690 22
305
260
2690 11
305
1
20 20
2090 1890
100
1600
2
450
260 260
2690 3300
100
2450
1
2
1600
1
20
305
2090 1890
450
2
2450
400
1
1
2
1600
1
2450
1600
1
450
2450
2890 2690
400
100
450
100
260
2890 2690
400
100
1890 22
(d)
455
Materials 2014, 7
5944 Figure 5. Cont. 100
305
2690 3300
305
1
1
2
2
20
20
1890 2800
390
455
455
455
1890 2800
1890
1890
11
11
11
2690
2690
1890
1890
22
22
22
22
(f)
455
390
390
390
2690
11
390
2690
(e)
100
400 1 2
2450
1 2
20 20
390
305
2450 1600
1 2
2090 1890
100
390
2690 3300
390
305
100
450
1600
1 2 20
450
2450
1 2
2090 1890
1600
100
400
400 1600
1 2
450
2450
2890 2690
100
450
100
400
2890 2690
100
(g)
(h)
Figure 6. Settings of the vertical reinforcement: (a) Wall thickness of 260 mm; and (b) Wall thickness of 390 mm.
(a)
(b)
2.2.2. Test Setup, Instrumentation and Procedure The test setup is shown in Figure 7. The specimen was connected to the top rigid girder and the concrete base. Vertical loading was applied firstly through a 1000 kN jack above the rigid distribution girder and kept constant. Then, lateral load reversals were applied to the top rigid girder by a servo actuator, which was supported by the strong reaction wall in the laboratory. The axial compression ratio in this experiment was taken as 0.2 for the specimens. Then, the applied vertical load was calculated by the following equation.
N nf m A
(3)
where N is the applied axial load, n is the experimental axial load ratio, fm is the average measured compressive strength of the RCB masonry, fm = 2.49 MPa, and A is the crosssectional area of the RCB masonry wall. In the test, both load and displacement controls were adopted at different loading stages. The loadcontrol method was adopted at the early loading stage, while the displacementcontrol method was after the yield point. Force sensors were set at the end of the vertical jack and the horizontal jack to monitor the loads. A displacement sensor was set at the middle of the rigid girder to monitor the horizontal displacement. All strains, displacements and loads were recorded and analyzed with the
Materials 2014, 7
5945
IMP (Interface Message Processor) data gathering system connected to the specimens. The cracking process of the wall was monitored visually during the tests. Figure 7. Test setup: (a) Schematic diagram; (b) Photograph.
(b)
(a) 2.2.3. Test Results Failure Patterns
The crack patterns and failure patterns of all specimens are shown in Figure 8. For the specimens without vertical reinforcement, MWA1, MWA2, MWA3 and MWA4, similar failure patterns could be observed: the horizontal cracks appeared firstly in the horizontal mortar between the bottom of the specimen and the concrete base and, then, developed gradually through the whole crosssection. The specimens showed the characteristics of shear sliding, and the bottom corner of the specimen crushed. As for the specimens with vertical reinforcement, MWB1, MWB2, MWB3 and MWB4, the horizontal cracks also appeared firstly in the horizontal mortar between the bottom of the specimen and the concrete base. Then, inclined cracks appeared in the specimen with an X shape. The inclined cracks developed gradually with the increase of the horizontal load and through the wall. The failure model was the shearcompression failure. As for the specimens with three vertical steel bars, MWB1 and MWB3, compared to the specimens with two vertical steel bars, MWB2 and MWB4, the middle vertical steel bar limited the development of the inclined cracks. The entire wall was divided into two areas, and in each area appeared inclined cracks with an X shape. Figure 8. Crack patterns and failure of the specimens: (a) MWA1; (b) MWB1; (c) MWA2; (d) MWB2; (e) MWA3; (f) MWB3; (g) MWA4; (h) MWB4.
(a)
(b)
(c)
(d)
Materials 2014, 7
5946 Figure 8. Cont.
(e)
(f)
(g)
(h)
LoadBearing Capacity Table 6 shows the cracking strength Fc, the effective yielding strength Fy and the lateral ultimate strength Fmax of the eight specimens; where Fc is the cracking load corresponding to the first occurrence of a crack appearing on the specimens and Fmax is the lateral ultimate loadbearing capacity, which is the maximum lateral load applied for the specimens. Rc, Ry and Rmax represent the ratio of the cracking strength, the yield strength and the ultimate strength of the specimen with vertical reinforcement to the specimens without vertical reinforcement, respectively. Table 6. Measured cracking strength, yield strength and ultimate strength. Specimen MWA1 MWB1 MWA2 MWB2 MWA3 MWB3 MWA4 MWB4
Fc (kN) 82.22 101.25 60.61 91.04 89.20 150.72 84.35 100.69
Rc 1.2315 1.5021 1.6896 1.1937
Fy (kN) 171.67 303.83 107.24 212.21 249.40 436.2 162.96 260.74
Ry 1.7698 1.9788 1.7190 1.6000
Fmax (kN) 220.87 380.80 131.00 252.07 326.53 496.88 195.55 305.25
Rmax 1.7241 1.9242 1.5270 1.5610
It can be seen from Table 6 that the walls with vertical reinforcement (specimens MWB1, MWB2, MWB3 and MWB4) showed better loadbearing capacity than those without vertical reinforcement (specimens MWA1, MWA2, MWA3 and MWA4). Deformation The measured displacements and displacement drifts of each specimen are listed in Table 7. All of the displacements were measured at the middle of the rigid girder, as shown in Figure 8. The values in Table 7 are defined as: δy is the yielding displacement, θy is the yielding displacement drift corresponding to δy, δu is the ultimate displacement and θu is the ultimate displacement drift corresponding to δu. The yielding displacement δy in Table 7 is obtained by the equivalent yield point determined on the skeleton curve. The socalled “equivalent energy method” [28] was adopted to determine the equivalent yield point, and its basic principle is illustrated in Figure 9. The ultimate state was defined by the point on the descending section of the envelope curve with 15% force degradation.
Materials 2014, 7
5947 Figure 9. Determination of the yield and ultimate points. Lateral Force F
A
Fmax 0.85Fmax
(2)
M U
Y (1) Area of (1)=Area of (2)
o
δy
δm
δu
Top displacement δ
Table 7. Measured yield displacement and ultimate displacement. Specimen MWA1 MWB1 MWA2 MWB2 MWA3 MWB3 MWA4 MWB4
Negative 3.74 5.44 5.25 7.16 4.38 6.89 5.85 4.79
δy (mm) Positive 2.24 4.19 2.70 4.16 4.85 6.15 3.39 7.41
Average 2.99 4.82 3.98 5.66 4.62 6.52 4.62 6.10
θy (%) δu (mm) θu (%) Average Negative Positive Average Average 0.19 8.35 8.75 8.55 0.48 0.30 15.19 21.18 18.19 1.02 0.24 8.47 10.41 9.44 0.53 0.35 12.15 16.74 14.45 0.81 0.29 12.78 13.55 13.17 0.74 0.41 16.59 21.25 18.92 1.06 0.29 14.52 16.46 15.49 0.87 0.38 20.54 23.76 22.15 1.12
The results in Table 7 showed that compared to the specimens without vertical reinforcement, MWA1, MWA2, MWA3 and MWA4, the yielding displacement δy of the specimens with vertical reinforcement, MWB1, MWB2, MWB3 and MWB4, increased by 61%, 42%, 41% and 32%, respectively. The ultimate displacement δu of the specimens with vertical reinforcement, MWB1, MWB2, MWB3 and MWB4, increased by 112%, 53%, 43% and 43%, respectively. The walls with vertical reinforcement showed better deformation capacity than those without vertical reinforcement. 2.2.4. Hysteretic Loops and Skeleton Curves The measured lateral loaddisplacement hysteretic loops and skeleton curves of the specimens are shown in Figures 10 and 11, respectively; where, δ is the displacement measured at the middle of the rigid girder and F is the lateral load. As shown in Figures 10 and 11: Compared to the specimens MWA1, MWA2, MWA3 and MWA4, the specimens with vertical reinforcement, MWB1, MWB2, MWB3 and MWB4, have the advantages of fuller hysteretic loops, slower stiffness degradation and higher elasticplastic deformation ability.
Materials 2014, 7
5948
Figure 10. Lateral loaddisplacement hysteretic loops of specimens: (a) MWA1; (b) MWB1; (c) MWA2; (d) MWB2; (e) MWA3; (f) MWB3; (g) MWA4; (h) MWB4.
(a)
(b)
(c)
(d)
(e)
(f)
(g)
(h)
Materials 2014, 7
5949
Figure 11. Lateral loaddisplacement skeleton curves of specimens: (a) MWA1 and MWB1; (b) MWA2 and MWB2; (c) MWA3 and MWB3; (d) MWA4 and MWB4.
(a)
(b)
(c)
(d)
2.2.5. Energy Dissipation The energy dissipation values were calculated by taking the average area surrounded by the positive and negative of the skeleton curve and the horizontal axis. The measured energy dissipation values are listed in Table 8, where A is the energy dissipation of the specimen and RA is the ratio of the energy dissipation between the specimen with vertical reinforcement and the specimen without vertical reinforcement. The results in Table 8 show that the measured energy dissipation capacity values of MWB1, MWB2, MWB3 and MWB4 are higher by 274%, 174%, 113% and 139%, respectively. This shows that the energy dissipation capacities of the specimens with vertical reinforcement are significantly greater than the specimens without vertical reinforcement. Table 8. Experimental results of energy dissipation. Specimen MWA1 MWB1 MWA2 MWB2 MWA3 MWB3 MWA4 MWB4
A (kN·mm) 3,054.91 11,436.13 2,042.21 5,611.24 7,091.88 15,102.86 4,712.14 11,274.29
RA 3.74 2.74 2.12 2.39
Materials 2014, 7
5950
2.2.6. Lateral Ultimate Strength Calculation The lateral ultimate strength of the RCB masonry wall with vertical reinforcement contains two parts. One is the contribution of the RCB wall without vertical reinforcement; the other is the contribution of concealed concrete columns. The shear strength equation of RCB walls embedded with vertical reinforcement is proposed as below and refers to the existing shear bearing capacity calculation equation, which is given by the design code of masonry structures, GB 50032011 [29]. V
1 [η γ RE
c
fvE ( A Ac )β ζ c ft Ac 0.08 f yc Asc ]
(4)
where γRE is the antiseismic adjusting factor of the bearing capacity, which reflects the influences of the concealed columns at the end of the wall section to the bearing capacity. fvE is the shear strength of RCB masonry fractured along the ladder section. A is the total crosssection area of the wall. Ac is the crosssection area of the midst concealed concrete column. Asc is the total crosssection area of the reinforcement in the middle of the concealed concrete column. ft is the concrete uniaxial tensile strength. fyc is the tensile strength of the vertical reinforcement. ηc is the constraint correction coefficient of the wall, which reflects the influences of the concealed columns in the middle of the wall section to the bearing capacity. ζc is the contribution coefficient of the middle concealed concrete column. β is the influence coefficient of the RCB masonry, considering the aspect ratio λ, β = 1.3 − 0.5λ (0.6 ≤ λ ≤ 1.0). As for the RCB masonry without vertical reinforcement, Ac = 0, ηc = 1, Asc = 0. The calculation of the lateral ultimate strength of eight specimens according to Equation (4) is shown in Table 9. It can be seen that the calculation results agree well with the experimental results. The proposed equation can be used to predict the lateral ultimate strength of the RCB masonry wall with vertical reinforcement. Table 9. The calculated values and measured values of lateral ultimate strength. Specimens MWA1 MWB1 MWA2 MWB2 MWA3 MWB3 MWA4 MWB4
Calculated (kN) 233.25 374.16 131.11 237.17 349.87 537.25 196.65 348.83
Measured (kN) 220.87 380.80 131.00 252.07 326.53 496.88 195.55 325.25
Errors (%) 5.61 1.74 0.08 5.91 7.14 8.12 0.56 7.25
3. FEM Analysis 3.1. Material Constitutive Models The damage plasticity model from the ABAQUS software was applied to simulate the concrete constitutive law. The stresslogarithmic strain relationship of concrete in code GB500102010 [30] was used here. The test values were obtained by the concrete cylinder compression test, and Poisson’s ratio was taken as 0.2.
Materials 2014, 7
5951
The stressstrain curve of a standard concrete cylinder subjected to a uniaxial compression is solved mathematically by Equation (5): Ec ε c,r f x ( x 0.143, 0.4 f c,r ) c,r Ec ε c,r nx ε σ ,x ,y y n 0.143 x 1 n ε c,r Ec ε c,r f c,r f c,r n 1 x x α ( x 1) 2 x x 1 c
(5)
where αc is the coefficient at the descent stage of the uniaxial compression stressstrain curve of concrete, fc,r is the representative value of uniaxial compressive strength of concrete, εc,r is the peak compressive strain of concrete corresponding to fc,r and Ec is the elastic modulus of concrete. In the numerical simulation, αc = 0.74, fc,r = 13.4 MPa, εc,r = 0.00133 and Ec = 2.55 × 104 MPa are based on the test concrete compressive strength and elastic modulus. The compressive stressstrain curve of concrete is plotted in Figure 12a. The compression damage factor dc can be calculated by Equation (6): d c 1 σ c Ec1 / (ε c ε cpl ) 1
σ c Ec1 ε cpl (1/ bc 1) σ c Ec1
ε c ε inc ε elc ε inc σ c Ec1
(6)
bc ε cpl / einc
where ε elc is the elastic compression strain, εinc is the inelastic compression strain and ε cpl is the plastic compression strain. In this paper, bc = 0.7. The “σε” formula for tension is given in the Equation (7): Ec ε t,r f x( x 1) t,r y x x 1 α t ( x 1)1.7 x
(7)
where αt is the coefficient at the descent stage of the uniaxial tension stressstrain curve of concrete, ft,r is the representative value of uniaxial tension strength of concrete and εt,r is the peak tension strain of concrete corresponding to ft,r. In the numerical simulation, αt = 0.7399, fc,r = 1.54 MPa and εc,r = 0.000604 are based on the test concrete tensile strength and elastic modulus. The tensile stressstrain curve of concrete is plotted in Figure 12b. The calculation of tension damage factor dt is given in Equation (8): dt 1
σ t Ec1 ε plt (1 / bt 1) σ t Ec1
ε t ε int ε elt ε int σ t Et1
(8)
bt ε plt / ε int
where, ε elt is the elastic compression strain, εint is the inelastic tension strain and ε plt is the plastic tension strain. In this paper, bt = 0.1.
Materials 2014, 7
5952
Figure 12. Constitutive law of concrete under uniaxial compression: (a) Compressive stressstrain curve; (b) Tensile stressstrain curve.
(a)
(b)
The constitutive law of the RCB wall: Integrated modeling by the plasticdamage model was based on ABAQUS. The compressive strainstress curve of RCB masonry obtained was based on Yang’s model [31]. The true values were obtained by the compression test on the RCB masonry and Poisson’s ratio was taken as 0.15. The “σcmεcm” formula for the compression of RCB masonry is given in Equation (9): Em ε cm x( x 0.365, σ 0.67 f cm ) f cm y , η Em / ( f cm / ε cm ) η x x 0.365 η η1 1 (η 1) x
(9)
where fcm is the representative value of the uniaxial compressive strength of RCB masonry, εcm is the peak compressive strain corresponding to fcm and Em is the elastic modulus of RCB masonry. In the numerical simulation, fcm = 2.49 MPa, εcm = 0.003 and Em = 2400 MPa are based on the test masonry strength and elastic modulus. The constitutive low of RCB masonry under uniaxial compression is shown in Figure 13. Figure 13. Constitutive law of RCB masonry under uniaxial compression.
The tensile softening uses the method based on fracture energy; where σ Itu f tm , f tm is the uniaxial tension strength of the RCB masonry, f tm 0.141/
f 2 [16] and f2 is the compressive strength of the
Materials 2014, 7
5953
mortar. The fracture energy GfI was taken as 20 N·m−1 [32]. The postfailure stressfracture energy curve in the descent stage is shown in Figure 14. Figure 14. Postfailure stressfracture energy curve in the descent stage for RCB masonry. σtI
σtuI GIf Uu0=2GIf /σtuI o
Uu0
The “plasticity” model from ABAQUS software was adopted to simulate the reinforcement law. The stressstrain curve is plotted in Figure 15. Each stressstrain curve, made up of two linear portions, represents the character of a bare mild steel bar; where the modulus Es is the elastic modulus of the reinforcement and the modulus E′ is the deformation modulus at the strain hardening stage, E′ = 0.01Es. The test yield strength and elastic modulus of the reinforcement were adopted in the paper, and Poisson’s ratio was taken as 0.3. Figure 15. Stressstrain curve of reinforcement.
E'
σ
Fy
Es o
ε
3.2. Finite Element Analysis Model Solid element C3D8R was used for concrete and masonry wall, and truss element T3D2 was used for reinforcement. All of the interface models, including the wall to load beam, wall to base and concealed concrete column to wall, were composed by contact in the lateral axis and stickslip along the tangential axis. The “hard contact” model was adopted for the contact on the lateral axis and the “Coulomb friction” model for the stickslip along the tangential axis. The friction coefficient was taken as 0.7 according to the code GB50032011[29]. Reinforcements were all embedded in the concrete. The bottom of the base was fixed rigidly. A vertically distributed load was applied to the top of the rigid girder first and kept constant. Then, horizontal displacement was applied to a coupling node in the middle plane of the rigid girder. A typical finite element analysis model of MWB1 is shown in Figure 16.
Materials 2014, 7
5954
Figure 16. Finite element analysis model of MWB1: (a) Element mesh; (b) Loading and boundary conditions (BCs).
(a)
(b)
3.3. Finite Element Simulation Results and Analysis Figure 17 shows the comparison of lateral loaddisplacement skeleton curves between calculated values and measured values. It shows that the initial elastic stage of the calculated curves is in good agreement with that of the measured curves. Because of the complex damage process of masonry walls and the sliding, the relative error becomes higher in the elasticplastic stage. However, the overall trend and the bearing capacity are still in good agreement with the measured values. Figure 17. Comparison of lateral load displacement skeleton curves between calculated values and measured values: (a) MWA1; (b) MWB1; (c) MWA2; (d) MWB2; (e) MWA3; (f) MWB3; (g) MWA4; (h) MWB4.
(a)
(b)
(c)
(d)
Materials 2014, 7
5955 Figure 17. Cont.
(e)
(f)
(g)
(h)
3.4. Effect of Axial Compressive Stress Σy on Lateral LoadDisplacement Curves and Lateral Ultimate Strength The mechanical performances of two simulated specimens, namely simulated Specimen 1 and simulated Specimen 2, were analyzed under six compressive stress ratios by ABAQUS. The parameter of the simulated Specimen 1 was the same as the test specimen MWB1 with an aspect ratio of 0.6, and the simulated Specimen 2 was the same as the test specimen MWB2 with an aspect ratio of 1.0. The change rules of lateral loaddisplacement curves to axial compressive stress ratio σy/fm are analyzed, where σy is the axial compressive stress of the wall section and fm is the average compressive strength of RCB masonry. The calculated lateral loaddisplacement curves of the two simulation specimens under six compressive stress ratios are shown in Figure 18. Figure 18. The calculated lateral loaddisplacement curves under different σy/fm: (a) Simulated Specimen 1; (b) Simulated Specimen 2.
(a)
(b)
Materials 2014, 7
5956
Figure 18 shows that under a certain limit of compressive stress ratio, the lateral ultimate strength (Fmax) of the RCB masonry walls with vertical reinforcement grows with the increase of the compressive stress ratio by a slow growth rate. However, the ductility declines with the increase of the compressive stress ratio by a fast degradation rate. The compressive stress ratio has little effect on the initial elastic stiffness, but affects the stiffness degradation speed gradually during the elastic stage to the elasticplastic stage. The concluded ultimate strength (Fmax)compressive stress ratio (σy/fm) curves of the two simulation specimens under nine compressive stress ratios are shown in Figure 19. Figure 19. The concluded ultimate strength (Fmax)compressive stress ratio (σy/fm) curves.
Figure 19 shows that the lateral ultimate strength of the RCB wall with vertical reinforcement experiences the process from the increase stage to the decrease stage with the increase of the compressive stress ratio. As for the two simulated specimens, the ultimate strength increases with the increase of the compressive stress ratio when the compressive stress ratio is less than 0.7, but declines when the compressive stress ratio exceeds 0.7. 4. Conclusions Based on the tests and the analytical results, the following conclusions can be drawn: 1.
2.
3.
The failure patterns of the RCB masonry are similar to common clay brick masonry when subjected to axial compression. The elastic modulus and Poisson’s ratio of the RCB masonry increase gradually as the mortar strength increases. For the RCB masonry walls with vertical reinforcement, the concealed concrete columns are effective in restricting the deformations and cracks of the wall and inducing the failure patterns to transform from brittleness to ductility. Compared to the RCB masonry walls without vertical reinforcement, the RCB masonry walls with vertical reinforcement have the advantages of fuller hysteretic loops, a lighter pinch in the middle of the loops, slower stiffness degradation and stronger elasticplastic deformation ability. Under a certain limit of the compressive stress ratio, the lateral ultimate strength of the vertical reinforcement RCB masonry walls grows with the increase of the compressive stress ratio by a slow growth rate. However, the ductility declines by a fast degradation rate. The compressive stress ratio has little effect on the initial elastic stiffness, but affects the stiffness degradation speed gradually during the period from the elastic stage to the elasticplastic stage.
Materials 2014, 7 4.
5957
The RCB masonry walls with vertical reinforcement have the advantages of easy construction, lower cost and good seismic performance, so they can be a good choice for the seismic design of rural lowrise buildings.
Acknowledgments The authors gratefully acknowledge the financial support from the “Twelfth FiveYear” Plan projects supported by the National Science and Technology of China under Grant No. 2011BAJ08B02 and the Doctoral Fund of Innovation of Beijing University of Technology of China under Grant No. YB201305. Conflicts of Interest The authors declare no conflict of interest. References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13.
Xiao, J.Z.; Li, W.G.; Yu, H.F.; Xiao, H. An overview of study on recycled aggregate concrete in China (1996–2011). Constr. Build. Mater. 2012, 31, 364–383. Hansen, T.C. Recycling of Demolished Concrete and Masonry; RILEM Report No. 6; E&FN Spon: London, UK, 1992. Collins, R.J. The Use of Recycled Aggregates in Concrete; BRE Report, Building Research Establishment: Watford, UK, 1994. Mehta, P.K.; Monteiro, P.J.M. Concrete: Structures, Properties and Materials; Prentice Hall: Englewood Cliffs, NJ, USA, 1993. Sherwood, P.T. Alternative Materials in Road Construction:a Guide to the Use of Waste, Recycled Materials and ByProducts; Thomas Telford: London, UK, 1995. Collins, R.J.; Harris, D.J.; Sparkes, W. Blocks with Recycled Aggregate: BeamandBlock Floors; Building Research Establishment: Watford, UK, 1998. Poon, C.S.; Kou, S.C.; Lam, L. Use of recycled aggregates in molded concrete bricks and blocks. Constr. Build. Mater. 2002, 16, 281–289. Gu, S.; Chen, G.P.; Zhu, S.W. Mechanical analysis of the recycled concrete brick masonry wall under inplane load. Adv. Mater. Res. 2011, 250–253, 278–282. Cao, W.L.; Zhou, Z.Y.; Dong, H.Y.; Zhang, Y.B. Shaking table test study on recycled aggregate concrete brick structure with vertical reinforcement. J. Earthq. Eng. Eng. Vib. 2012, 32, 111–117. He, X.X.; Zhang, T. Experimental study on strength and other performance of solid concrete bricks made from recycled coarse aggregate. Appl. Mech. Mater. 2013, 357–360, 1212–1218. Guo, Z.G.; Sun, W.M.; Wang, J.; Chen, J.L.; Xu, Y.F. Experimental study on seismic behavior of recycled concrete perforated brick masonry. Adv. Mater. Res. 2011, 163–167, 1879–1882. He, X.X.; Zhang, T. Experimental study on drying shrinkage performance of solid concrete bricks made from recycled coarse aggregate. Adv. Mater. Res. 2013, 753–755, 762–770. Valdés, G.A.; Rapimán, J.G. Physical and mechanical properties of concrete bricks produced with recycled aggregates. Inf. Technol. 2007, 18, 81–88.
Materials 2014, 7
5958
14. Lourenco, P.B.; Rots, J. GA solution for the macromodeling of masonry structures. Proceeding of 11th International Brick/Block Masonry Conference, Shanghai, China, 14–16 October 1997; pp. 1239–1249. 15. Andreaus, U. Failure criteria for masonry panels under in plane loading. J. Struct. Eng. ASCE 1996, 1, 37–46. 16. Shi, C.X. Masonry Structure Theory and Design, 2nd ed.; Architecture & Industry Press of China: Beijing, China, 2003. (In Chinese) 17. Luo, W.K.; Zhu, X.C.; Liao, C.S. Correlation analysis of shearcompression correlation and the shear friction coefficient values. Eng. Mech. 1997, 2, 135–141. 18. Cai, Y.; Shi, C.X.; Ma, C.L.; Bao, T. Study of the masonry shear strength under shearcompression action. J. Build. Struct. 2004, 25, 118–123. 19. Liu, G.Q.; Shi, C.X.; Huang, L. Analyses of the failure criteria of masonry in compressionshear. J. Hunan Univ. Nat. Sci. 2007, 34, 19–23. 20. Chinese National Standards. Common Portland Cement; GB1752007; Standards Press of China: Beijing, China, 2008. (In Chinese) 21. Chinese National Standards. Standard for Test Method of Basic Mechanics Properties of Masonry; GB/T501292011; Architecture & Industry Press of China: Beijing, China, 2011. (In Chinese) 22. Francis, A.T.; Horinan, C.B.; Jerrems, L.E. The effect of joint thickness and other factors on the compressive strength of brick work. In Proceedings of the 2nd International Brick Masonry conference, StokeonTrent, UK, 12–15 April 1971; pp. 31–37. 23. Hilsdorf, K.H. Masonry materials and their physical properties. In Proceedings of International Conference on Structural Design of Tall Concrete and Masonry Buildings, ASCE, New York, NY, USA, August 1972; pp. 981–999. 24. Hendry, A.W. Structural Brickwork; John Wiley and Sons.: New York, NY, USA, 1981. 25. Онишшк, Л.И. Research of Masonry Structure; Sciences Press: Beijing, China, 1955. (In Chinese) 26. Grimm, C.T. Strength and related properties of brick masonry. J. Struct. Div. 1975, 101, 217–232. 27. British Standards. Code of Practice for Structural Use of MasonryPart 1: Structural Use of Unreinforced Masonry; BS56281; BSI: London, UK, 1992. 28. Guo, Z.H. Reinforced Concrete Theory and Analyze; Press of Tsinghua University: Beijing, China, 2003. 29. Chinese National Standards. Code for Design of Masonry Structures; GB500032011; Architecture & Industry Press of China: Beijing, China, 2012. (In Chinese) 30. Chinese National Standards. Code for Design of Concrete Structures; GB500102010; Architecture & Industry Press of China: Beijing, China, 2011. (In Chinese) 31. Yang, W.Z. Constitutive relationship model for masonry materials in compression building structure. Build. Struct. 2008, 38, 80–82. 32. Yue, J.G.; Qian, J.; Wu, K.; Fu, Q.S.; Pan, Y. A modified plastic damage model for masonry structure. Chin. Q. Mech. 2012, 33, 146–152. © 2014 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/3.0/).